Received 30 January 2014 Accepted 27 June 2014 Published 16 July 2014

Correspondence and requests for materials should be addressed to R.W.W. (Roger. [email protected])

Absence of Evidence ? Evidence of Absence: Statistical Analysis of Inclusions in Multiferroic Thin Films Michael Schmidt1,2, Andreas Amann1,3, Lynette Keeney1, Martyn E. Pemble1,2, Justin D. Holmes1,2,4, Nikolay Petkov1 & Roger W. Whatmore1,2,5 1

Tyndall National Institute, University College Cork, ‘Lee Maltings’, Dyke Parade, Cork, Ireland, 2Department of Chemistry, University College Cork, Cork, Ireland, 3School of Mathematical Sciences, University College Cork, Ireland, 4Centre for Research on Adaptive Nanostructures and Nanodevices, Trinity College Dublin, Dublin 2, Ireland, 5Department of Materials, Royal School of Mines, Imperial College London, South Kensington Campus, London SW7 2AZ, UK.

Assertions that a new material may offer particularly advantageous properties should always be subjected to careful critical evaluation, especially when those properties can be affected by the presence of inclusions at trace level. This is particularly important for claims relating to new multiferroic compounds, which can easily be confounded by unobserved second phase magnetic inclusions. We demonstrate an original methodology for the detection, localization and quantification of second phase inclusions in thin Aurivillius type films. Additionally, we develop a dedicated statistical model and demonstrate its application to the analysis of Bi6Ti2.8Fe1.52Mn0.68O18 (B6TFMO) thin films, that makes it possible to put a high, defined confidence level (e.g. 99.5%) to the statement of ‘new single phase multiferroic materials’. While our methodology has been specifically developed for magnetic inclusions, it can easily be adapted to any other material system that can be affected by low level inclusions.

or N.P. ([email protected] tyndall.ie)

‘‘A

bsence of Evidence is not Evidence of Absence’’ is a truism which confounds many analytical assertions. The confident statement of certainty: ‘‘There was nothing there’’ leads to the obvious retort: ‘‘How do you know?’’. In many analyses, especially those using microscopes (optical or electron), it is only possible to look at restricted volumes, and the smaller the inclusion, or defect, or the lower the level of the impurity being sought, the smaller the volume that can reasonably be examined. The absence of any evidence for second phases, defects or impurities in these volumes can lead to the erroneous conclusion (perhaps driven by wishful thinking) that there are none in the sample as a whole, when in fact all that can be asserted with certainty was that there was nothing in the volumes examined at the limit of resolution for the technique used. And yet all is not lost, because if the detection thresholds of a particular method are well understood, the volumes examined are known and one makes some justifiable assumptions about the size distributions of second phase particles being sought, then one can apply statistical methods to determine the confidence level that surrounds such a statement. In other words, one can convert the assertion of ‘‘certainty-ofabsence’’ to one which gives a level of probability that the density of the sought-for impurity or second phase inclusion is below a certain critical level. Conversely, it is possible to apply such methods to the design of experiments which will yield any required level of confidence. For example, it is possible to say that if one requires a confidence of 99.5% that the density of a certain impurity or defect of known composition and/or size is below a certain critical level in a specimen, then given the sensitivities of the analytical methodologies being used, the statistical analysis can be used to determine how large a total volume needs to be examined. If one considers different examples of materials analysis, there are different cases according to whether one is searching for impurity elements in a simple, single element material like silicon, trying to detect inclusions which are widely different in composition/structure from the parent matrix or looking for second phases that are similar in composition and/or structure to the parent. If the material is a pure element like silicon, for instance, claims with respect to a given level of purity can be verified relatively easily by using a host of different techniques such as SIMS (secondary ion mass spectrometry) and the level of impurities can be determined down to the level of ppb1–4. On the other hand, there are scanning methods which can locate inclusions and structural defects5,6, but, as commonly used, these are generally limited to detecting a minimum amount of 1–2 weight% of a particular inclusion type7. Atom probe tomography (APT)8 and scanning transmission electron microscopy (STEM)

SCIENTIFIC REPORTS | 4 : 5712 | DOI: 10.1038/srep05712

1

www.nature.com/scientificreports coupled with energy dispersive X-ray spectroscopy (EDS/EDX)9 and/ or electron energy loss spectroscopy (EELS)10,11 provide techniques which can resolve single atoms spatially and elementally, but are limited to very small sample volumes (areas of a few nm2 within a single atomic layer such as graphene film for example). Hence they cannot deal with a statistical distribution of small numbers of such entities dispersed over tens of mm3. There is a significant probability that the examination of a small volume of material at the high detail needed to see such very small inclusions may easily miss them, simply because they are not present in the particular volume of material examined. In such a case it is prejudicial to say that such defects or inclusions are not present in the sample - one can only put a probability upon them for their density being below a certain critical level. On the other hand, an aggressive search for new materials is in progress and the development of single-phase multiferroic (simultaneously ferromagnetic and ferroelectric) oxides is a good example of this. These materials are of considerable interest for future memory and sensing applications12–18. Here, the assertion that a new material is a single-phase, room-temperature multiferroic may be confounded by the presence of second-phase ferromagnetic inclusions that may have formed during the sample preparation. This is the single most critical factor in the analysis of such materials because the magnetic properties of the sample overall are highly susceptible to the presence of such inclusions. The difficulty in excluding second phase inclusions as being responsible for any observed ferromagnetism of a given sample is that some of the elements used to form the main phase could easily be responsible for formation of a ferromagnetic second phase. The differences between main and second phases could be in stoichiometry and/or crystal structure and both factors may have influence on the magnetic behaviour. This report demonstrates an original methodology for the detection, localization and quantification of second phase inclusions in thin Aurivillius type films. Even when the compositional differences between inclusion and main phase are rather subtle, our methodology provides a viable approach to not only identifying the inclusions but also to their localization and further in-depth structural investigation. Additionally, we develop a dedicated statistical model applied to the design of the analytical (EDX) measurements and demonstrate its application to the analysis of Bi6Ti2.8Fe1.52Mn0.68O18 (B6TFMO) thin films. We present a detailed account of the sample preparation, transmission electron microscopy (TEM) and energy dispersive X-ray analysis (EDX) that was necessary to put a high, defined confidence level (.99.5%) to the statement of ‘new single phase multiferroic material’. While this methodology has been developed specifically to identify magnetic second phase inclusions, it can easily be applied to other material systems, given that the analytical measurement and statistical model is adapted to the special case, thus making the developed methodology comprehensively applicable. It closes an existing gap in the analysis of materials, between atomic scale analysis and the detection of obvious large scale (micron size) inclusions. Due to the fast pace of development in the hard- and software for elemental detection when using the electron beam as a probe, further development of the presented methodology can be sought by introducing necessary automation19,20.

Statistical Analysis Our analysis requires a number of concepts from statistics, which we now introduce. We will start by analyzing the statistical significance of a single measurement of a given sample volume and at a fixed resolution, and then proceed to evaluate a series of measurements at varying volumes and resolutions. Finally we show how to conclude with a high, pre-set statistical confidence level (e.g. 99.5%) that a physical effect (which in the case at hand is the magnetic remanence of the sample) is not caused by undetected inclusions or defects. SCIENTIFIC REPORTS | 4 : 5712 | DOI: 10.1038/srep05712

Single measurement. In general, it is impossible to prove with certainty that no inclusions exist in a given sample, unless the whole sample is scanned for inclusions. In order to nevertheless obtain statistically significant results, we use the method of statistical inference through the refutation of a null hypothesis. In the case at hand we assume that the level of concentration of a particular impurity exceeds a certain level, and then show that this assumption does not hold with a certain statistical level of confidence. More specifically, let us first assume that a particular type of second (or impurity) phase inclusion is present in the sample at a known (volume) density r and let us further assume that the individual inclusions do not interact with each other and are therefore independently distributed. We measure the number of inclusions found in a scan of a small volume V, as shown schematically in figure 1. The probability P(N, r) of finding precisely N inclusions is given by the Poisson distribution PðN,rÞ~

ðrV ÞN {rV e : N!

ð1Þ

In particular, the probability that no inclusions are present in a scanned volume V is given by Pð0,rÞ~e{rV : If we now fix a desired confidence level c (in our case c 5 99.5%) and define the value rNu implicitly via N X P m,rNu ~1{c

ð2Þ

m~0

then it follows from (1) that for any value of the impurity density r bigger than ruN, the probability of finding N or fewer inclusions within a volume V is below 1 2 c 5 0.5%. In the special case that no inclusions were found equation (2) can be solved explicitly and yields r0u ~

{lnð1{cÞ 5:3 < , V V

If a performed scan of the volume V yields N or fewer inclusions, we can therefore conclude that rvrNu

ð3Þ

with a confidence of c 5 99.5%. Subject to this confidence level, the rNu defined in equation (3) establishes an upper bound for the unknown inclusion density r. The grain size distribution function. So far we have assumed that there exists only one type of inclusion. In reality, inclusions can vary in grain size and composition. For simplicity, let us first study the case where the chemical composition of the inclusion is fixed (for example, Fe3O4 as worst case scenario in our case) and all inclusions are spherical. However, we do not make any prior assumptions with regards to the inclusion grain size. We can thus introduce a grain size

Figure 1 | Schematic illustration of a scan of a volume V (small yellow box). What conclusions can we draw, if no inclusions (red balls) are detected during the scan? 2

www.nature.com/scientificreports distribution function pG(d), such that for small Dd the quantity pG(d)Dd is the density of inclusions with diameters in the range [d, d 1 Dd]. We can now generalize the upper bound (3) for the case of a size dependent distribution function as follows: assume that a scan of a certain volume V established that there are N inclusions present which are larger than a minimal detectable size dm. Then we can conclude that ? ð dqpG ðqÞvrNu

Effect of inclusions on remanent magnetisation. In the previous paragraph we established an upper limit of the volume fraction of inclusions in thin films. However, our aim is to establish an upper bound on the contribution of such inclusions on a measurable quantity. For multiferroic materials, the relevant quantity is the remanent magnetisation, which we will discuss now. Given the bound on the volume fraction, we can define the maximal contribution to the remanence from inclusions with diameters in the interval [dk, dk21] as Mr,k,u ~Qk,u Mr,F ðdk{1 Þ

dm

with confidence level c 5 99.5%. Series of measurements. So far we have considered only one volume scan. In practice, any analysis will employ a number (K) of scans with different volume sizes Vk possessing different minimal detectable grain sizes dk where the index k 5 1, …, K enumerates the individual scans starting at large dk (i.e. dk . dk11) that yielded Nk or fewer inclusions. Furthermore we assume that there is a physical upper bound d0 . d1 on the grain size. For a given grain size distribution function pG(d) we can define the density of inclusions bigger than dk via dðo rk ~ pG ðqÞdq

Here Mr,F(d) is the remanent magnetization of pure Fe3O4 grains of diameter d. For simplicity we assume that Mr,F(d) vanishes for ,5 nm. Furthermore we set Mr,F(d) 5 10 emu/g for 5 nm , d , 20 nm and Mr,F(d) 5 20 emu/g for d . 20 nm which are conservative estimates. Finally we can establish an upper bound for the total contribution from inclusions to the remanent magnetisation as ( ) K X Mr,u ~ max Wk Mr,k,u W1 ,,WK

K X

m~0

The probability of finding fewer than Nk inclusions in a sequence of scans from k 5 1, …, K is given by the product of the individual probabilities

k~1

with a confidence level c. Here, the parameters W1, …, WK fulfill the constraint

dk

Then the probability of finding Nk or fewer inclusions in one particular scan k is given by Nk X Pk ðNk Þ~ Pðm,rk Þ

ð5Þ

Wk ~1:

k~1

Therefore we can conclude that the contribution to the magnetization remanence from inclusions Mr has an upper bound Mr,u ~ max fMr,k,u g k~1...K

with confidence c 5 99.5%.

P~P1 ðN1 ÞP2 ðN2 Þ PK ðNK Þ: Let us now assume that all individual scans establish that no inclusion was detected larger than the respective minimal grain size, dk. This is the case for the application at hand and therefore will now be discussed in more detail. The probability for this zero outcome is given by Pð0Þ~P1 ð0ÞP2 ð0Þ PK ð0Þ: The volume fraction Qk of inclusions between sizes dk and dk21 can be calculated from the grain size distribution pG(d) assuming spherical inclusions ð dk{1 ð dk{1 4 q 3 p 3 Qk ~ dqpG ðqÞ p ƒ dqpG ðqÞ dk{1 : 3 2 6 dk dk In this step we have employed the worst case scenario that the weight of the grain size distribution function is located at the large inclusion sizes. It therefore follows that there is an upper limit Qk,u on the volume fraction Qk of inclusions with diameter in the interval [dk, dk21] given by {d 3 d3 p Qk vQk,u ~ Pk k{1 lnð1{cÞ